metal induced crystallization - induced crystallization 463 oxide interface layer, depending on the...
Post on 07-Mar-2018
Embed Size (px)
Metal Induced Crystallization Ahamad Mohiddon Mahamad and Ghanashyam Krishna Mamidipudi
School of Physics, University of Hyderabad, Hyderabad, India
1. Introduction Polycrystalline silicon thin films have attracted the attention of semiconductor industries in the past few decades due to their wide applications in thin film transistors, solar cells, display units and sensors (Schropp & Zeman, 1998; Choi et al., 2005; Mahan et al., 2008). Polycrystalline Si thin films are generally fabricated by crystallizing amorphous Si (a-Si) thin films, because these can render larger grains compared to the conventional poly Si film deposition. As a consequence, a variety of methods for lowering the crystallization temperature of a-Si have been developed. Excimer laser annealing is one of the promising ways to achieve large grain size poly Si films at lower substrate temperatures. Its high costs and nonuniform grain size, however, are significant obstacles that prevent its wide use (Parr et al., 2002). The other promising technique is the solid phase crystallization method. But this technique is essentially a high-temperature process and many substrates, including most forms of glass, cannot withstand the thermal processing. In order to achieve lower costs and have a wider range of application, inexpensive materials such as glass and special polymers have to substitute quartz or Pyrex substrates. In the case of glass substrates, all of the processing steps need to be limited to temperatures below 550 C. The other known technique is rapid thermal annealing (RTA). In RTA infrared radiation is used as a heating source, and has the advantage of the high heating speed (up to 60 C/s) that reduces the crystallization time. In RTA radiation is applied in pulses to heat the sample without heating the glass substrate (which is transparent to the infrared radiation). However, the grain size obtained in the crystallization of a-Si is also in the range of a few micrometers.
In an effort to reduce the crystallization temperature and crystallization time, and to increase the grain size, metal-induced crystallization (MIC) has been investigated as an alternative crystallization process for thin-film device fabrication. The MIC process involves the deposition of a-Si films on top of which a layer of suitable metal is deposited. This bilayer of metal and Si is then annealed in a furnace at temperatures ranging from 150 to 700 C for durations between one minute to several hours leading to crystallization of the a-Si. As a result the Si nanocrystals grow in the metal/metal silicide/metal oxide matrix and their growth rate depends on the annealing conditions of the bilayer. Thus, to grow the Si nanocrystals, both thermodynamics and kinetics of the process have to be understood in detail. In the MIC process, metals like aluminum, nickel, gold, silver etc are used to decrease the crystallization temperature below 700 C. Among the metals employed for the study of the MIC (Jin et al.,1999; Kumar et al.,2007; Kumar et al.,2008; Mohiddon & Krishna, 2011), the preferred metal up to date has been nickel (Ni) due to its low residual metal
Crystallization Science and Technology
contamination in the poly-Si region (Wang & Wong, 2001). The mobility and the transfer characteristics of the poly Si TFT are improved by reducing the leakage current caused by the metal agents. To achieve this, metal-induced lateral crystallization (MILC) has been introduced. Ni induced MILC TFTs are now widely used in large display applications. Large number of metals have been investigated to crystallize the a-Si at possible low temperature. These metals are classified in to two groups basing on the mechanism they follow in crystallizing the a-Si matrix. One group of metals forms eutectic with a-Si (follows Layer exchange mechanism) and the other reacts with a-Si and forms silicide. The eutectic phase forming metals can produce extended continuous poly-Si films with large grain size of 10 m (Oliver & Hartmann, 2000). However, these metals contaminate the so produced c-Si and degrade its properties. Thus, the search for metals that would lead to crystallization of a-Si thin film at low temperatures and also reduce the contamination is a subject of recent research.
The aim of this review is to present an overview of the current state of understanding of the mechanisms involved in MIC and to discuss some of the recent work of the current authors in this area. The motivation is to crystallize a-Si films using metals that have not been investigated in detail so far, in addition to Ni which is a well studied metal used in the MIC process. The two other metals that were selected for this study are Tin (Sn) and Chromium (Cr). The former is known to form a eutectic alloy with the Si whereas the latter is a silicide/oxide forming metal, similar to Nickel. Furthermore, results on two different types of geometries are presented; the first involves the deposition of metal on top of the a-Si film, while in the second geometry the a-Si film is deposited on top of the metal film. This provides very interesting insights in to the mechanisms that cause crystallization of a-Si.
2. Mechanisms of metal induced crystallization The main mechanisms of metal induced crystallization are discussed in this section.
2.1 Layer exchange mechanism
The proposed formation of poly-Si films on foreign substrates by eutectic forming metals relies on the overall layer exchange of adjacent Si and metal films during the transformation of amorphous to polycrystalline Si. The phenomenon is named as layer exchange mechanism. The general driving force behind metal-induced crystallization is the reduction of the free energy of the silicon material during the transformation of the amorphous to the crystalline phase. When a-Si is in contact with certain metals, electronic screening of the covalent bonding in the Si material occurs, which weakens the Si bonds, and therefore, facilitates the inter diffusion of the metal and silicon atoms (Hiraki, 1980). The representatives of the eutectic forming metals are Au, Ag and Al. Aluminum-induced crystallization [AIC] is extensively studied metal to form extended continuous poly-Si films of large-grained material on glass, which is desirable for thin film solar cells.
The AIC comprises the diffusion of Si atoms into the Al layer, which occurs due to the fact that adjacent Al and Si layers are not in thermal equilibrium at elevated temperatures. According to the Al/Si phase diagram, up to 1.5 at.% of Si can be dissolved in Al at temperatures below the eutectic temperature of 577 C (Murray & McAlister, 1984). The initial interaction of the Al and a-Si layers involves the partial dissolution of the Al or Si
Metal Induced Crystallization
oxide interface layer, depending on the layer sequence, to allow the inter diffusion of the materials. The Si oxide layer is transformed by the Al into a mixture of Al oxide and an AlxSi phase. This newly formed AlxSi phase provides a diffusion channel for the Si and Al atoms (Nast & Wenham, 2000). The evaporated Al films are of polycrystalline nature, there are four different diffusion paths available for the diffusion of the Si atoms. 1) Diffusion inside the Al grains, 2) Diffusion along Al grain boundaries, 3) Diffusion along the Al/a-Si interfaces, and 4) Diffusion along the glass/Al interface.
The diffused Si atoms start crystallizing near the Al/a-Si interface. The Al grain boundaries are preferential nucleation sites for the dissolved Si atoms, since they are the sites of low critical free energy for nucleus formation. According to the random successive nucleation model, at early stage of crystallization, Si nuclei are formed at preferred sites located at the Al/Si interface. The released heat (crystallization energy and strain energy) leads to rise the local temperature in ambient regions. The temperature field propagates fast, since the thermal diffusion is faster than the atomic diffusion, so that the heat flow can stimulate new nuclei appearing randomly in nearby region. These nuclei of the next generation also produce a local temperature rise. This process repeats many time during annealing, resulting in a fractal formation.
Silicon atoms, dissolved in the Al layer, have a high mobility and, hence, diffuse quickly within the film and/or along the interfaces towards the growing Si grains (McCaldin & Sankur, 1971). It is this fast growth within the Al layer compared to any other growth normal to the layer structure that leads to the formation of a continuous poly-Si film. At an early stage of the crystallization process the newly formed Si grains within the Al matrix are far apart and do not influence each other. The nucleation rate strongly depends on the defects and grain boundaries in the Al layer as well as the temperature and corresponding silicon concentration. Si solute depletion occurs up to the effective diffusion distance in the vicinity of the growing grain (Zener, 1949). In this region the possibility of new nucleation decreases with increasing depletion towards the advancing Al/Si grain interface. When the effective diffusion distances of adjacent grains begin to overlap, competition for the available Si atoms dissolved in the Al layer occurs. At this point, the possibility of new nuclei formation decreases. This type of crystallization pattern, where isolated grains start to interfere at an early stage of the process, is different to solid-phase crystallization of amorphous silicon (Spinella et al., 1998).
The grain-size distribution is dependent on the ratio of the grain growth to the nucleation rate. This ratio increases with decreasing annealing temperature (Nast & Wenham, 2000). The decrease in grain growth due to a lower a